# Functional Materials from Biomass-Derived Terpyridines: State of the Art and Few Possible Perspectives

Jérôme Husson

► To cite this version:

Jérôme Husson. Functional Materials from Biomass-Derived Terpyridines: State of the Art and Few Possible Perspectives. International Journal of Molecular Sciences, 2024, 25 (16), pp.9126. 10.3390/ijms25169126. [https://doi.org/10.3390/ijms25169126]

HAL Id: hal-04681074

https://hal.science/hal-04681074v1

Submitted on 30 Aug 2024

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
<figure><img src="image_2.png" /></figure>

Review

# Functional Materials from Biomass-Derived Terpyridines: State of the Art and Few Possible Perspectives

Jérôme Husson

<figure><img src="image_3.png" /></figure>

Institut UTINAM, UMR CNRS 6213, Université de Franche-Comté, 16 Route de Gray, F-25000 Besançon, France;
jerome.husson@univ-fcomte.fr

**Abstract:** This review focuses on functional materials that contain terpyridine (terpy) units, which can be synthesized from biomass-derived platform chemicals. The latter are obtained by the chemical conversion of raw biopolymers such as cellulose (e.g., 2-furaldehyde) or lignin (e.g., syringaldehyde). These biomass-derived platform chemicals serve as starting reagents for the preparation of many different terpyridine derivatives using various synthetic strategies (e.g., Kröhnke reaction, cross-coupling reactions). Chemical transformations of these terpyridines provide a broad range of different ligands with various functionalities to be used for the modification or construction of various materials. Either inorganic materials (such as oxides) or organic ones (such as polymers) can be combined with terpyridines to provide functional materials. Different strategies are presented for grafting terpy to materials, such as covalent grafting through a carboxylic acid or silanization. Furthermore, terpy can be used directly for the elaboration of functional materials via complexation with metals. The so-obtained functional materials find various applications, such as photovoltaic devices, heterogeneous catalysts, metal-organic frameworks (MOF), and metallopolymers. Finally, some possible developments are presented.

**Keywords:** catalysts; dye-sensitized solar cells; ligands; metal complexes; metal-organic frameworks; oligopyridines

<figure><img src="image_4.png" /></figure>

check for
updates

**Citation:** Husson, J. Functional Materials from Biomass-Derived Terpyridines: State of the Art and Few Possible Perspectives. *Int. J. Mol. Sci.* **2024**, *25*, 9126. https://doi.org/10.3390/ijms25169126

Academic Editor: Raphaël Schneider

Received: 1 July 2024

Revised: 20 August 2024

Accepted: 21 August 2024

Published: 22 August 2024

<figure><img src="image_5.png" /></figure>

**Copyright:** © 2024 by the author. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## 1. Introduction

In 1932, Morgan and Burstall [1] described the first synthesis of 2,2':6',2''-terpyridine (Figure 1). Since then, a plethora of terpyridine derivatives has been prepared. This can be explained by the fact that terpyridine derivatives (terpys) are ligands able to form complexes with various metals. Varying the nature of the metallic center and/or substituents onto the ligands offers the possibility to prepare a broad range of different substances. The so-obtained compounds find applications in numerous fields [2,3], such as in medicinal chemistry [4], biological probes [5], sensors [6], or as energy storage devices [7], just to name a few.

<figure><img src="image_6.png" /><figcaption>**Figure 1.** Chemical structure and atom-numbering of 2,2':6',2''-terpyridine.</figcaption></figure>

In the late 1990s, Anastas and Warner introduced the twelve principles of green chemistry as guidelines to make chemical processes more environmentally friendly [8]. One of the principles is to use renewable feedstocks, such as biomass, instead of oil-derived substances. In fact, biomass is renewable, contrary to crude oil. Furthermore, the use
of crude oil has detrimental effects on the environment [9]. Consequently, turning to biomass as a source of chemicals can help mitigate environmental problems [10]. This review emphasizes using biomass-derived platform chemicals in synthesizing terpyridine ligands as a green chemistry approach. The utilization of these ligands in the fabrication of functional materials is also presented. Finally, applications of the so-obtained materials are described.

## 2. Preparation of Functional Materials from Biomass-Derived Terpyridines

Many synthetic pathways are available for the preparation of terpyridine derivatives [11–13]. Most of them rely on the Kröhnke reaction (Scheme 1), which involves the reaction of two equivalents of an acetylpyridine derivative with an aldehyde in a basic medium and in the presence of an ammonia source [14].

<figure><img src="image_7.png" /><figcaption>**Scheme 1.** Reaction scheme for the Kröhnke synthesis of terpyridines.</figcaption></figure>

Many aldehydes (Figure 2) are available through the conversion of biomass [15,16]. For instance, furan-derived aldehydes (2-furaldehyde, 2,5-diformylfuran, 5-halomethylfurfural, etc.) are obtained by chemical conversion of cellulose or hemicellulose [17–24], while vanillin and syringaldehyde derivatives can be obtained by the transformation of lignin [25–31].

<figure><img src="image_8.png" /><figcaption>**Figure 2.** Selected examples of biomass-derived aldehydes obtained from cellulose, hemicellulose, or lignin.</figcaption></figure>

Therefore, it is no surprise that biomass-derived aldehydes can be used as starting materials in the preparation of terpys to be used in functional materials.

### 2.1. Materials for Photovoltaic Applications

Dye-sensitized solar cells (DSSC) are devices that turn solar light into electricity [32]. Firstly, described in 1991 [33], these photoelectrochemical systems rely on a functional material [34], which combines a wide bandgap semiconductor (generally TiO₂) and an organic or organometallic sensitizer (the “dye”). Classically, such solar cells are composed of two electrodes, one of them being coated with the functional material (Figure 3).
<figure><img src="image_9.png" /><figcaption>**Figure 3.** Schematic representation of a DSSC.</figcaption></figure>

Upon light irradiation, the dye (D) undergoes an excited state (D*) from which an electron is injected onto the semiconductor, thus generating the electrical current and leaving the sensitizer in an oxidized state. This requires the sensitizer to be regenerated in its ground, reduced state by recovering an electron from the counter-electrode. To achieve this, a redox shuttle ($I_3^−/I^−$, for example) is used to transfer electrons from one side of the system to another. This closes the cycle, which can be repeated [35]. The efficiency of such solar cells ($η$) is defined as the ratio between the energy received from light and the electrical energy generated by the system. This efficiency is expressed as a percentage, and currently, the most efficient devices have $η$ around 13% [36].

Amongst the variety of sensitizers that have been evaluated in DSSCs [37], terpyridines play an important role [38,39]. For instance, the so-called “black-dye” (1) (Figure 4) has been, for many years, one of the most efficient sensitizers [40,41].

<figure><img src="image_10.png" /><figcaption>**Figure 4.** Chemical structure of “Black-Dye” (1). Tetrabutylammonium counter-cations omitted.</figcaption></figure>

This ruthenium (II) terpyridine complex features carboxylate groups, which ensure a good anchorage onto $TiO_2$ nanoparticles, as well as favoring electron injection, thus forming a valuable functional-material for DSSC applications [42]. Preparing “black-dye” requires the prior synthesis of 4,4',4"'-tricarboxy-2,2':6',2"'-terpyridine ligand (2). The original route towards compound 2 is based on a two-step process (Scheme 2) from 4-ethylpyridine. Nevertheless, this pathway suffers low yield, high energy demand, usage of toxic reagents, and a high level of chemical waste.
<figure><img src="image_11.png" /></figure>

Reagents and conditions:

i. Pd/C
170°C, 9 days, 20 %

ii. K₂Cr₂O₇
H₂SO₄, 36 %

<caption>**Scheme 2.** Original route to 4,4',4''-tricarboxy-2,2':6',2''-terpyridine (2).</caption>

Alternatively, molecule 2 can be prepared from biomass-derived furfural in three steps, as depicted in Scheme 3 [43,44]. The initial step consists on the synthesis of keto-derivative (3) from commercially available ethyl isonicotinale and a Minisci-type reaction [45]. The former is then converted to furan-substituted terpy 4 through a reaction with furfural under Kröhnke's conditions. Finally, the furan ring is degraded into carboxylate using a potassium permanganate-mediated oxidation.

<figure><img src="image_12.png" /></figure>

Reagents and conditions:

i. Paraldehyde; tBuOOH; FeSO₄, 7H₂O; CF₃COOH
CH₃CN, reflux, 4 h, 81 %

ii. Furfuraldehyde; KOH; aq. NH₃
Ethanol, room temperature, 24 h, 64 %

iii. KMnO₄; KOH
H₂O, room temperature, 24 h, 93 %

<figure><img src="image_13.png" /><figcaption>**Scheme 3.** "Furan" alternative route to 4,4',4''-tricarboxy-2,2':6',2''-terpyridine.</figcaption></figure>

When compared to the original route to (2), the "furan" alternative ticks several principles of green chemistry [46]:

- 1) Prevention of wastes;

- 3) Less hazardous chemical synthesis;

- 6) Design for energy efficiency;

- 7) Use of renewable feedstock.

In fact, the amount of waste generated during the process, as measured by the E-factor [47], is divided by a factor of approximately three (106 vs. 336 g·g⁻¹, respectively). Secondly, the furan route avoids the use of toxic chromium (VI) salts. Thirdly, this process is less energy-intensive, and finally, it uses a biomass-derived reagent (furfural). With this new, more environmentally friendly method for the preparation of ligand **2**, many other metal complexes incorporating it were synthesized and evaluated in DSSCs [48–52].

Biomass-derived furfural can also be used for the preparation of terpyridines **5–7**, which can undergo oxidation of the furan ring to carboxylic acid moieties similarly to the preparation of **2** [43,53,54]. This provides new ligands **8, 9**, and **10** (Scheme **4**), which can be incorporated into various metal-based sensitizers for DSSCs [55–59].
<figure><img src="image_14.png" /><figcaption>**Scheme 4.** Synthetic pathways for the preparation of ligands 5–10 from biomass-derived furfural.</figcaption></figure>

It is worth mentioning that the furan-oxidation methodology can be extended to the preparation of ligands for the fabrication of sensitizers that do not contain terpyridines, but bipyridine or bipyrimidine instead [60–62]. Moreover, furan oxidation can be carried out directly onto a preformed complex [63], thus allowing the synthesis of dyes **11–13** (Scheme 5) starting from biomass-derived terpy 5 [64–66].

<figure><img src="image_15.png" /><figcaption>**Scheme 5.** Conversion of biomass-derived terpyridine 5 into sensitizers **11–13** (counter-anions omitted).</figcaption></figure>

Apart from being an important intermediate in the preparation of carboxy-substituted dyes, terpyridine 5 was also used for the preparation of metal-based sensitizers in which the furan heterocycle is unaltered. Molecule 5 was combined with 4,4'-dicarboxy-2,2'-bipyridine to afford heteroleptic complex 14 (Figure 5), which was assessed as a dye in
DSSCs. Anchorage onto TiO₂ is effected via the bipyridine part of the complex thanks to -COOH groups. Unfortunately, the efficiency of the device so-fabricated is limited to a poor 0.13% [67].

<figure><img src="image_16.png" /><figcaption>**Figure 5.** Chemical structure of complex 14.</figcaption></figure>

As can be seen, furfural has been widely used in the preparation of terpyridine-based dyes. Nevertheless, other biomass-derived chemicals have also been used in the conception of such sensitizers. For instance, 3,4,5-trimethoxybenzaldehyde (15) can be used to prepare terpyridine 16 (Figure 6) using the Kröhnke reaction [68]. 3,4,5-trimethoxybenzaldehyde can be obtained from naturally occurring syringaldehyde, vanillin, or gallic acid [69–71]. Thus, one can consider ligand 15 as a biomass-derived compound.

<figure><img src="image_17.png" /><figcaption>**Figure 6.** Chemical structures of 3,4,5-trimethoxybenzaldehyde (15) and 4'-(3,4,5-trimethoxypenyl)-2,2':6',2''-terpyridine (16).</figcaption></figure>

Terpyridine **16** is then converted in three steps to sensitizer **17** (Scheme 6). This heteroleptic Ru(II) complexes is then adsorbed onto TiO₂, and the obtained functional material is evaluated in a DSSC. The device reaches 4.62% efficiency [72].

In the above-mentioned examples, all sensitizers are prepared from aldehydes via the Kröhnke reaction. However, it is also possible to prepare dye from non-aldehyde biomass-derived platform chemicals, such as Tiglic acid, a naturally occurring substance that can be isolated from many different plants [73]. Heck cross-coupling reaction with 4'-bromo-2,2':6',2''-terpyridine afforded ligand **18**. The latter is used for the synthesis of Ru(II)-homoleptic complex **19** (Scheme 7). Although no solar cell was made and characterized in the study, the photophysical properties of **19** were studied and suggested a possible application in DSSCs owing to its high molar absorption coefficient [74].
<figure><img src="image_18.png" /><figcaption>**Scheme 6.** Synthetic pathway towards photosensitizer **17**.</figcaption></figure>

<figure><img src="image_19.png" /><figcaption>**Scheme 7.** Synthetic pathway towards complex **19**.</figcaption></figure>
## 2.2. Materials for Catalysis

Terpyridine derivatives are widely employed in the field of catalysis [3,75]. Functional materials that incorporate biomass-derived terpyridines have been investigated as catalysts, especially in heterogeneous catalysis. In fact, such functional materials are generally insoluble in the reaction medium, thus allowing their recovery at the end of the reaction.

Quite similar to DSSCs (see above Section 2.1), complex **20** (Figure 7) can be grafted onto platinized titanium dioxide. The obtained functional material can be used as a photocatalyst for the generation of $H_2$ in aqueous media [76]. Upon irradiation, the Pt-complex injects an electron onto $TiO_2$. This photogenerated electron is driven to Pt-particules, where it achieves proton reduction to $H_2$. Regeneration of the sensitizer to its ground state is achieved via a sacrificial electron donor (triethanolamine).

<figure><img src="image_20.png" /><figcaption>**Figure 7.** Schematic representation of the photocatalyst based on complex **20**.</figcaption></figure>

This material is able to produce $H_2$ upon irradiation at $λ > 410$ nm but with low rates and few turnovers. A possible explanation for these facts is the oxidative degradation of the complex onto the surface.

Terpyridine **8** is also used to prepare complex **21** (Figure 8). Thanks to the carboxylic acid group, compound **21** can be anchored onto silica, thus making a heterogeneous catalyst that can be used for the hydrodeoxygenation of aromatic alcohols [77]. Different binding modes are proposed between the molecular part of the catalyst and the silica material. These include electrostatic interactions, hydrogen, and covalent bondings.

<figure><img src="image_21.png" /><figcaption>**Figure 8.** Structure of heterogeneous catalyst (left) based on complex **21** and the model hydrodeoxygenation reaction (right) that it catalyzes.</figcaption></figure>

This catalyst is easily prepared by simply soaking silica particles in a DMF solution of the complex. This point is advantageous due to potential large-scale applications. The efficiency of this catalyst in the model reaction was measured in different solvents
ranging from polar ones (e.g., methanol) to apolar ones (e.g., dodecane). Best efficiencies are achieved in non-polar solvents. In fact, such solvents are able to stabilize catalyst bonding onto silica. Furthermore, these solvents do not coordinate with the Pd-center, thus preserving catalyst efficiency.

Anisaldehyde and 4-hydroxybenzaldehyde are two chemicals that can be isolated from plants or via biomass transformation [78–81]. Conversion of these two aldehydes into terpyridines **22** and **23** (Figure 9) is again effected using Kröhnke's reaction. Furthermore, it is also possible to prepare compound **23** from **22** through methyl-ether cleavage.

<figure><img src="image_22.png" /><figcaption>**Figure 9.** Chemical structures of terpyridine **22** (left) and **23** (right) synthesized from anisaldehyde and 4-hydroxybenzaldehyde, respectively.</figcaption></figure>

Ligand **22** can be used for the preparation of a Ru(II)-heteroleptic complex that is grafted onto multi-walled carbon nanotubes (MWCNT), thus providing a material (Figure 10) that is able to catalyze water splitting for the production of oxygen [82].

<figure><img src="image_23.png" /><figcaption>**Figure 10.** Ru(II)-appended MWCNT-functional material for water splitting to O₂.</figcaption></figure>

Fabrication of this material is a two-step process starting from 4-methyl-2,2'-bipyridine-4'-carbaldehyde [83]. The latter is first grafted onto the nanotube via a Prato reaction [84]. Then, the metallic center is introduced onto the material through a reaction with Ru(21)Cl₃. Electrochemical measurements indicate that the chloride ligand is replaced by water during the oxygen evolution reaction (OER), thus making the reactant (water) close to the active center. Additionally, the nanostructure of the catalyst makes active centers readily accessible. Finally, the covalent grafting ensures a better transfer of electrons. All these properties combined make this material an efficient catalyst for water splitting.

Grafting of ligand **23** onto inorganic materials (such as silica or iron oxide) proceeds using the general protocol outlined in Scheme 8. Firstly, the oxide is activated by silanization (step 1) with an alkoxysilane derivative [85]. Especially, (3-chloropropyl)trimethoxysilane is used since it contains a C-Cl bond prone to nucleophilic substitution. The reaction of activated oxide with ligand **23** forms a covalent bond between oxide particles and the terpyridine unit (step 2). Finally, the complexation of the terpyridine unit with various metals (step 3) leads to functional materials for catalytic applications.
<figure><img src="image_24.png" /><figcaption>**Scheme 8.** General protocol for the functionalization of various oxides with terpyridine **23**.</figcaption></figure>

This methodology is employed for the preparation of numerous heterogeneous catalysts to be used in many different reactions (Table 1).

<table><caption>**Table 1.** Oxide-based heterogeneous catalysts prepared via silanization with (3-chloropropyl) trimethoxysilane and reaction with **23**.</caption><thead><tr><th>Nature of Oxide</th><th>Complexed Metal (M)</th><th>Catalyzed Reaction</th><th>References</th></tr></thead><tbody><tr><td rowspan="2">Fe<sub>3</sub>O<sub>4</sub></td><td>Pd</td><td>•Suzuki<br>•Heck</td><td>[86]</td></tr><tr><td>Cu</td><td>•Huisgen<br>•C-S coupling</td><td>[87]</td></tr><tr><td>MnFe<sub>2</sub>O<sub>4</sub></td><td>Mo</td><td>•Epoxidation</td><td>[88]</td></tr><tr><td rowspan="3">Graphene Oxide</td><td rowspan="3">Pd</td><td>•Suzuki</td><td rowspan="3">[89]</td></tr><tr><td>•Heck</td></tr><tr><td>•C-N coupling<br>•C-O coupling</td></tr><tr><td>SiO<sub>2</sub></td><td>Nb</td><td>•Phtalimides<br>synthesis</td><td>[90]</td></tr></tbody></table>

A similar methodology was employed for preparing a polymer-stabilized palladium catalyst suitable for Suzuki and Heck reactions [91]. This catalyst is loaded onto iron oxide for magnetic recovery. The activation of iron oxide particles is effected with 3-(trimethoxysilyl) propyl methacrylate, leaving a material with pendant reactive acrylate moieties. The latter is reacted with terpyridine **24** (Figure 11), which features a C=C bond, in a radical polymerization reaction. This creates a polymeric network containing pendant terpyridines. This terpyridine-functionalized material is finally complexed with palladium
(PdCl₂). Since the complexation step is carried out in ethanol, Pd(II) is reduced to Pd(0) to afford the active catalyst as Pd nanoparticles. Interestingly, terpyridine 24 is obtained by esterification between biomass-derived ligand 23 and another biomass-derived chemical, namely Itaconic acid [92]. The active material can be recycled up to four times and its efficiency is similar to other Pd-based nanocatalysts.

<figure><img src="image_25.png" /><figcaption>**Figure 11.** Chemical structure of bis-terdentate ligand 24.</figcaption></figure>

It is worth mentioning that compound 24 can also be used as a co-monomer with trimethylolpropane triacrylate to prepare a terpyridine-functionalized copolymer without any supporting oxide. This polymeric material can be loaded with palladium to afford a catalyst suitable for C-C coupling reactions [93].

Nucleophilic displacement of a chlorine atom onto a is also exemplified in the preparation of an iron terpyridine-containing resin, the latter being used as a catalyst for epoxide opening [94]. A chloromethylated polystyrene-based resin is treated with 23, thus providing a material with pendant terpyridine units, which are complexed with Fe(III), to afford the catalyst (Scheme 9).

<figure><img src="image_26.png" /><figcaption>**Scheme 9.** Preparation of a terpyridine complex polystyrene material (perchlorate counter-anions omitted).</figcaption></figure>

In the previous examples, the terpyridine system is chemically bonded to the material. Nevertheless, it is also possible to physically bond the ligand through electrostatic interactions. This approach is used to prepare a polystyrene (PS)-based material containing
palladium [95]. Firstly, 4-hydroxybenzaldehyde reacts with propanesultone, thus allowing sulfonic acid to contain aldehyde **25**. The latter is then reacted with 2-acetylpyridine to afford ligand **26**, which is reacted with an amino-functionalized PS resin. Proton exchange between the sulfonic acid and the amine group leads to charged species (positively charged PS resin and negatively charged ligand). Electrostatic interactions ensure the anchoring of the ligand onto the material. Finally, complexation with palladium affords an active material suitable for C-C coupling reactions (Scheme 10).

<figure><img src="image_27.png" /><figcaption>**Scheme 10.** Synthetic pathway towards a PS-terpyridine material suitable as catalyst for C-C coupling.</figcaption></figure>

All reactions are carried out in water, making this material an interesting catalyst in view of green chemistry. Furthermore, despite being non-covalently bonded, this material exhibits an interesting chemical stability as demonstrated by the low level of Pd leaching, which remains below 3 µg.L⁻¹ (except for the Heck reaction, which shows a small leaching level of 5 ppm).

### 2.3. Metallopolymers, Metal–Organic Frameworks (MOFs) and Polyoxometalates (POMs)

Metallopolymers and MOFs are materials that include coordinated metals in their structures [96,97]. Owing to the ability of terpyridines to easily form complexes with many metals, it is no surprise that such ligands are widely used for the preparation of such materials [98]. Some examples of the utilization of biomass-derived terpy ligands for the construction of MOF or metal-containing polymers have been reported in the literature so far.

Terpyridine **5** is used for the synthesis of heteroleptic Ru(II) complex **27**, which features a thiophene heterocycle. This complex can be electrochemically polymerized thanks to the presence of the thiophene ring, which provides a material that is deposited onto the surface of an electrode as a thin film (Scheme 11) [99]. The backbone of the material is a polythiophene chain with pendant Ru(II) complexes. Nevertheless, no application for the so-obtained material is reported, as described in this paper, which was solely intended to study the properties of the complex.
<figure><img src="image_28.png" /><figcaption>**Scheme 11.** Preparation of a metallopolymer via electropolymerization of complex 27.</figcaption></figure>

Similarly, 4,4',4'',4''-tricarboxy-2,2':6',2''-terpyridine 2 can be combined with a terthiophene-substituted terpyridine to afford a Ru(II) complex (28) (Figure 12) that can undergo electropolymerization giving a metallopolymer polymer with pendant Ru(II) metallic centers [100].

<figure><img src="image_29.png" /><figcaption>**Figure 12.** Chemical structure of complex 28.</figcaption></figure>

The so obtained metallopolymer was tested as a sensitizer in DSSCs but exhibited poor performance. Fast deactivation of the excited state could be the reason for such inefficiency.

Metal-containing polymer 29 (Figure 13) can be obtained in four steps from 4-hydroxybenzaldehyde. This metallopolymer is water soluble thanks to the presence of -OH groups in the side chains. Owing to the presence of $Eu^{3+}$ ions in its structure, polymer 29 is luminescent. The luminescence decreases in the presence of pyrophosphate anion, thus making this polymer a probe for pyrophosphate monitoring in living cells [101].
<figure><img src="image_30.png" /><figcaption>**Figure 13.** Chemical structure of metallopolymer 29.</figcaption></figure>

The sensing of pyrophosphate anion is affected by measuring the luminescence of the material at λ = 613 nm. The molecular mechanism that is involved is due to the ability of pyrophosphate anions to coordinate with Eu³⁺ ions. This results in the abstraction of Eu³⁺ from the polymer matrix and, in turn, a reduction in the luminescence of the material.

Metal-containing polymer **30** (Figure 14) is obtained in a similar way [102]. It was evaluated as an active material in light-emitting diodes (LED) and as a temperature sensor.

<figure><img src="image_31.png" /><figcaption>**Figure 14.** Chemical structure of metallopolymer 30.</figcaption></figure>

The emissive properties of this material are explained by the transfer of energy be-
tween the different constituent parts of the polymer. In particular, transfers between the
tetraphenylethene part and the Eu³⁺ ion.

The three previous examples are metal-containing polymers where the metal is in a
pendant position. However, it is also possible for the metallic centers to be included in
the polymer backbone. In these cases, the polymer chain is built up by the formation of
coordinative bonds. Synthesis of such a material is generally performed using polytopic
ligands, which bear multiple coordination sites [103]. Terpyridine **31** (Figure 15) is a ditopic
ligand that is prepared in three steps from 4'-carboxy-2,2':6',2''-terpyridine (8).
<figure><img src="image_32.png" /><figcaption>**Figure 15.** Chemical structure of terpyridine 31.</figcaption></figure>

The originality of compound 31 is the presence of both a terdentate site (terpyridine part of the molecule) and a bidentate site (pyridyl-triazole part of the molecule). This allows the coordination of different metals at each site and the preparation of mixed-metals coordination polymers (Figure 16) [104].

<figure><img src="image_33.png" /><figcaption>**Figure 16.** Coordination polymer obtained from ligand 31 and mixed metals.</figcaption></figure>

Metal 1 can be selected between Fe(II), Co(II), or Ru(ii), while metal 2 can be either Cu(I) or Ag(I). These metallopolymers were studied for their electrochemical and magnetic properties.

Ligand 4 (Scheme 3) is also considered a polytopic ligand since it possesses the terpyridine scaffold as well as carboxylic acids, which can also be used for coordinating metals. This terpyridine is used for the construction of a 3D porous Zn(II) MOF [105]. The latter is obtained through the complexation of two independent Zn(II) ions in two different coordination modes (Figure 17). The first Zn ion (Zn1) is in a distorted octahedral geometry involving the three nitrogen atoms of one molecule of 3 and three oxygen atoms from two other ligands. The second Zn ion (Zn2) is five coordinated by using the three nitrogen atoms of one molecule of 3 and two oxygen atoms from two other ligands. The obtained MOF exhibits fluorescence property, which is quenched in the presence of nitro compounds. In fact, the latter can interact with the MOF structure through π-π interactions and/or H-bonding, resulting in fluorescence quenching. Therefore, this MOF could be used as a nitro-compounds sensor.
<figure><img src="image_34.png" /><figcaption>**Figure 17.** Coordination modes of ligand 4.</figcaption></figure>

Additionally, this MOF can be carbonized to afford a porous carbon-based material for gas adsorption [106].

All terpyridines described in the present review so far are 2,2′:6′,2″-terpyridine derivatives. Nevertheless, 4,2′:6′,4″-terpyridines, although being less common than 2,2′:6′,2″-terpyridines, are useful bricks for the construction of MOFs or metallopolymers [107–109]. Especially 4,2′:6′,4″-terpyridines are used for the coordination of two metallic centers instead of one in the case of 2,2′:6′,2″-terpyridine derivatives. This two metals ligation is effected via the two outer pyridine rings (Figure 18).

<figure><img src="image_35.png" /><figcaption>**Figure 18.** Coordination modes of 2,2′:6′,2″-terpyridines (**left**) and 4,2′:6′,4″-terpyridines (**right**).</figcaption></figure>

Terpyridine **32** (Figure 19) is obtained from anisaldehyde and 4-acetylpyridine using the classic Kröhnke method [110]. This ligand can be coordinated with CuI, thus forming a 2D MOF with Cu<sub>2</sub>I<sub>2</sub> clusters as nodes.

<figure><img src="image_36.png" /><figcaption>**Figure 19.** Structure of terpyridine **32** (**left**) and its coordination mode to Cu<sub>2</sub>I<sub>2</sub> clusters (**right**).</figcaption></figure>

The 2D nets so obtained are interdigitated, thus forming a 3D porous MOF with 1D channels. The 3D structure is stabilized by π-π and CH-π interactions, and the voids in the supramolecular structure are able to accept guest molecules. The inclusion of small molecules into the channels leads to the modification of the optical properties of the material, making it an optical sensor for various substances.
Finally, combining terpyridine **32** with various carboxylated co-ligands and Co(II) ions is a strategy that gives rise to various MOF architectures such as 2D sheets, 3D frameworks, and 3D interpenetrated frameworks [111]. These different MOFs were evaluated for their gas adsorption as well as for their magnetic properties.

Polyoxometalates (POM) are inorganic building blocks that possess interesting properties [112]. These materials find applications in many fields, such as catalysis [113], photo(electro-) chemical applications [114], or as sensors [115], just to name a few. POM can be functionalized with a pendant terpyridine moiety using ligand **8** as a starting material [116]. Firstly, compound **8** is converted to ester **33**. Then, the latter is transformed into amide **34** via reaction with Tris. Hydroxy groups onto **34** then allow the grafting of terpyridine moieties onto various POMs (Scheme 12).

<figure><img src="image_37.png" /><figcaption>**Scheme 12.** Synthetic pathway towards ligand **34**. Inset: schematic representation of a POM-terpyridine material (adapted from reference [116]).</figcaption></figure>

The properties of the materials obtained were studied, and although the paper does not describe direct applications of these POMs, a possible one could be as a photoactive material.

**3. Conclusions and Perspectives**

As demonstrated above, biomass-derived chemicals are versatile reagents for the synthesis of terpyridine ligands to be incorporated into functional materials. Figure 20 highlights the various possibilities that are offered for the preparation of biomass-derived terpyridine ligands.
<figure><img src="image_38.png" /><figcaption>**Figure 20.** Summary of the different biomass-derived terpyridine ligands discussed in this review and their interconnections.</figcaption></figure>

Given the almost infinite possibilities of compounds that can be obtained by combining a terpyridine ligand with a metal, it is entirely reasonable to believe that biomass-derived terpyridines will continue to be used for the construction of functional materials. Recent scientific literature seems to support this. Indeed, several recently published articles report the use of terpyridines in the manufacture of functional materials, particularly in the field of electrical energy storage [117–121]. Although these recently described ligands are not biomass-derived, it is entirely possible to imagine that the terpyridines shown in the present paper could be incorporated into such functional materials. This is all the more likely as electricity storage issues are widely studied in the context of sustainable development [122] and confirmed by a very recent example of the utilization of terpyridine 2 for the fabrication of a material to be applied in this field [123].

Another perspective for using these biosourced terpyridines could be the valorization of carbon dioxide, again with a view to sustainable development [124]. Indeed, the use of terpyridine-metal complexes in this field of application is already well documented [125–133]. Thus, it is reasonable to believe that biosourced terpyridines could play an important role in this area of application.

Finally, the last potential field of applications (i.e., for biomass-derived terpyridines) that will be mentioned in the present paper is the biomedical domain. Many terpyridine-based materials have been evaluated in this field. The latter can be used both for their
cytotoxic properties [134–137], their anti-bacterial properties [138,139], and even as biosensors just to name a few [140,141].

Of course, this list of potential applications is not exhaustive. Many others can be imagined. This is why it is very likely that biomass-derived terpy ligands will continue to be widely studied by the community of chemists and materials scientists in the future.

**Funding:** This research received no external funding.

**Institutional Review Board Statement:** Not applicable.

**Informed Consent Statement:** Not applicable.

**Data Availability Statement:** No new data were created or analyzed in this study.

**Conflicts of Interest:** The author declares no conflicts of interest.

## References

1. Morgan, S.G.; Burstall, F.H. Dehydrogenation of pyridine of anhydrous ferric chloride. *J. Chem. Soc. 1932*, **1**, 20–30. [CrossRef]

2. Schubert, U.S.; Hofmeier, H.; Newkome, G.R. *Modern Terpyridine Chemistry*; Wiley-VCH: Weinheim, Germany, 2006.

3. Schubert, U.S.; Winter, A.; Newkome, G.R. *Terpyridine-Based Materials: For Catalytic, Optoelectronic and Life Sciences Applications*; Wiley-VCH: Weinheim, Germany, 2011.

4. Cummings, S.D. Platinum complexes of terpyridine: Interaction and reactivity with biomolecules. *Coord. Chem. Rev.* **2009**, *253*, 1495–1516. [CrossRef]

5. Abhijnakrishna, R.; Magesh, K.; Ayushi, A.; Velmathi, S. Advances in the Biological Studies of Metal-Terpyridine Complexes: An Overview From 2012 to 2022. *Coord. Chem. Rev.* **2023**, *496*, 215380. [CrossRef]

6. Bhattacharya, S.; Pal, P.; Baitalik, S. Design of molecular sensors and switches based on luminescent ruthenium-terpyridine complexes bearing active methylene and triphenylphosphonium motifs as anion recognition sites: Experimental and DFT/TDDFT investigation. *Dalton Trans.* **2024**, *53*, 1307–1321. [CrossRef]

7. Laschuk, N.O.; Ebralidze, I.I.; Zenkina, O.V. Polypyridine-based architectures for smart electrochromic and energy storage materials. *Can. J. Chem.* **2023**, *101*, 400–417. [CrossRef]

8. Anastas, P.T.; Warner, J.C. *Green Chemistry: Theory and Practice*; Oxford University Press: Oxford, UK, 1998.

9. Cherubini, F. The biorefinery concept: Using biomass instead of oil for producing energy and chemicals. *Energy Conv. Manag.* **2010**, *51*, 1412–1421. [CrossRef]

10. Arias, A.; Feijoo, G.; Moreira, M.T. Biorefineries as a driver for sustainability: Key aspects, actual development and future prospects. *J. Clean. Prod.* **2023**, *418*, 137925. [CrossRef]

11. Heller, M.; Schubert, U.S. Syntheses of functionalized 2,2':6',2''-terpyridines. *Eur. J. Org. Chem.* **2003**, *6*, 947–961. [CrossRef]

12. Fallahpour, R.A. Synthesis of 4'-substituted-2,2':6',2''-terpyridines. *Synthesis* **2003**, *2*, 155–184. [CrossRef]

13. Thompson, A.M.W.C. The synthesis of 2,2':6',2''-terpyridine ligands- versatile building blocks for supramolecular chemistry. *Coord. Chem. Rev.* **1997**, *160*, 1–52. [CrossRef]

14. Kröhnke, F. Synthesis using pyridinium salts. *Specific synthesis of pyridines and oligopyridines*. *Synthesis* **1976**, *1*, 1–24. [CrossRef]

15. Luterbacher, J.S.; Martin Alonso, D.; Dumesic, J.A. Targeted chemical upgrading of lignocellulosic biomass to platform molecules. *Green Chem.* **2014**, *16*, 4816–4838. [CrossRef]

16. Isikgor, F.H.; Remzi Becer, C. Lignocellulosic biomass: A sustainable platform for the production of bio-based chemicals and polymers. *Polym. Chem.* **2015**, *6*, 4497–4559. [CrossRef]

17. Jaswai, A.; Pratap Singh, P.; Mondai, T. Furfural—A versatile, biomass-derived platform chemical for the production of renewable chemicals. *Green Chem.* **2022**, *24*, 510–551. [CrossRef]

18. Gomez Millan, G.; Hellsten, S.; Llorca, J.; Luque, R.; Sixta, H.; Balu, A.M. Recent Advances in the Catalytic Production of Platform Chemicals from Holocellulosic Biomass. *ChemCatChem* **2019**, *11*, 2022–2042. [CrossRef]

19. Zhang, Z.-H.; Sun, Z.; Yuan, T.-Q. Recent Advances in the Catalytic Upgrading of Biomass Platform Chemicals Via Hydrotalcite-Derived Metal Catalysts. *Trans. Tianjin Univ.* **2022**, *28*, 89–111. [CrossRef]

20. Weng, R.; Lu, X.; Ji, N.; Fukuoka, A.; Shrotri, A.; Li, X.; Zhang, R.; Zhang, M.; Xiong, J.; Yu, Z. Taming the butterfly effect: Modulating catalyst nanostructures for better selectivity control of the catalytic hydrogenation of biomass-derived furan platform chemicals. *Catal. Sci. Technol.* **2021**, *11*, 7785–7806. [CrossRef]

21. Li, X.; Zhang, L.; Wang, S.; Wu, Y. Recent Advances in Aqueous-Phase Catalytic Conversions of Biomass Platform Chemicals Over Heterogeneous Catalysts. *Front. Chem.* **2020**, *7*, 948. [CrossRef]

22. Dedes, G.; Karnaouri, A.; Topakas, E. Novel Routes in Transformation of Lignocellulosic Biomass to Furan Platform Chemicals: From Pretreatment to Enzyme Catalysis. *Catalysts* **2020**, *10*, 743. [CrossRef]

23. Irshad, M.; Lee, S.; Choi, E.; Kim, J.W. Efficient Synthetic Routes of Biomass-derived Platform Chemicals. *Appl. Chem. Eng.* **2019**, *30*, 280–289.
24. Serrano-Ruiz, J.C.; Luque, R.; Sepulveda-Escribano, A. Transformations of biomass-derived platform molecules: From high added-value chemicals to fuels via aqueous-phase processing. *Chem. Soc. Rev.* **2011**, *40*, 5266–5281. [CrossRef] [PubMed]

25. Jiang, L.; Wang, C.-G.; Chee, P.L.; Qu, C.; Fok, A.Z.; Yong, F.H.; Ong, Z.L.; Kai, D. Strategies for lignin depolymerization and reconstruction towards functional polymers. *Sustain. Energy Fuels* **2023**, *7*, 2953–2973. [CrossRef]

26. Yang, W.; Ding, H.; Puglia, D.; Kenny, J.M.; Liu, T.; Guo, J.; Wang, Q.; Ou, R.; Xu, P.; Ma, P.; et al. Bio-renewable polymers based on lignin-derived phenol monomers: Synthesis, applications, and perspectives. *SusMat* **2022**, *2*, 535–568. [CrossRef]

27. Costa, C.A.E.; Vega-Aguilar, C.A.; Rodrigues, A.E. Added-Value Chemicals from Lignin Oxidation. *Molecules* **2021**, *26*, 4602. [CrossRef] [PubMed]

28. Liu, C.; Wu, S.; Zhang, H.; Xiao, R. Catalytic oxidation of lignin to valuable biomass-based platform chemicals: A review. *Fuel Process. Technol.* **2019**, *191*, 181–201. [CrossRef]

29. Lee, S.; Monnappa, A.K.; Mitchell, R.J. Biological activities of lignin hydrolysate-related compounds. *BMB Rep.* **2012**, *45*, 265–274. [CrossRef]

30. Sun, Z.; Fridrich, B.; de Santi, A.; Elangovan, S.; Barta, Z. Bright Side of Lignin Depolymerization: Toward New Platform Chemicals. *Chem. Rev.* **2018**, *118*, 614–678. [CrossRef] [PubMed]

31. Walton, N.J.; Mayer, M.J.; Narbad, A. Vanillin. *Phytochemistry* **2003**, *63*, 505–515. [CrossRef]

32. Kalyanasundaram, K. *Dye-Sensitized Solar Cells*; CRC Press: Boca Raton, FL, USA, 2010.

33. O'Regan, B.; Grätzel, M. A low-cost, high-efficiency solar cell based on dye-sensitized colloidal TiO₂ films. *Nature* **1991**, *353*, 737–740. [CrossRef]

34. Tontapha, S.; Uppachai, P.; Amornkitbamrung, V. Fabrication of Functional Materials for Dye-sensitized Solar Cells. *Front. Energy Res.* **2021**, *9*, 641983. [CrossRef]

35. Hagfeldt, A.; Boschloo, G.; Sun, L.; Kloo, L.; Pettersson, H. Dye-Sensitized Solar Cells. *Chem. Rev.* **2010**, *110*, 6595–6663. [CrossRef]

36. Rahman, S.; Haleem, A.; Siddiq, M.; Hussain, M.K.; Qamar, S.; Hameed, S.; Waris, M. Research on dye sensitized solar cells: Recent advancement toward the various constituents of dye sensitized solar cells for efficiency enhancement and future prospect. *RSC Adv.* **2023**, *13*, 19508–19529. [CrossRef] [PubMed]

37. Yen, Y.-S.; Chou, H.-H.; Chen, Y.-C.; Hsu, C.-Y.; Lin, J.T. Recent developments in molecule-based organic materials for dye-sensitized solar cells. *J. Mater. Chem.* **2012**, *22*, 8734–8747. [CrossRef]

38. Saccone, D.; Magistris, C.; Barbero, N.; Quagliotto, P.; Barolo, C.; Viscardi, G. Terpyridine and Quaterpyridine Complexes as Sensitizers for Photovoltaic Applications. *Materials* **2016**, *9*, 137. [CrossRef] [PubMed]

39. Rees, T.W.; Baranoff, E. Ruthenium complexes with tridentate ligands for dye-sensitized solar cells. *Polyhedron* **2014**, *82*, 37–49. [CrossRef]

40. Nazeeruddin, M.K.; Péchy, P.; Grätzel, M. Efficient panchromatic sensitization of nanocrystalline TiO₂ films by a black dye based on a trithiocyanato-ruthenium complex. *Chem. Commun.* **1997**, *18*, 1705–1706. [CrossRef]

41. Nazeeruddin, M.K.; Péchy, P.; Renouard, T.; Zakeeruddin, S.M.; Humphry-Baker, R.; Comte, P.; Liska, P.; Cevey, L.; Costa, E.; Shklover, V.; et al. Engineering of Efficient Panchromatic Sensitizers for Nanocrystalline TiO₂-Based Solar Cells. *J. Am. Chem. Soc.* **2001**, *123*, 1613–1624. [CrossRef]

42. Reynal, A.; Forneli, A.; Palomares, E. Dye structure-charge transfer process relationships in efficient ruthenium-dye based sensitized solar cells. *Energy Environ. Sci.* **2010**, *3*, 805–812. [CrossRef]

43. Dehaudt, J.; Husson, J.; Guyard, L. A more efficient synthesis of 4,4',4"'-tricarboxy-2,2':6',2"'-terpyridine. *Green Chem.* **2011**, *13*, 3337–3340. [CrossRef]

44. Husson, J.; Dehaudt, J.; Guyard, L. Preparation of carboxylate derivatives of terpyridine via the furan pathway. *Nat. Protoc.* **2014**, *9*, 21–26. [CrossRef]

45. Duncton, M.A.J. Minisci reactions: Versatile CH-functionalizations for medicinal chemists. *Med. Chem. Commun.* **2011**, *2*, 1135–1161. [CrossRef]

46. Anastas, P.; Eghbali, N. Green Chemistry: Principles and Practice. *Chem. Soc. Rev.* **2010**, *39*, 301–312. [CrossRef] [PubMed]

47. Sheldon, R.A. The E factor at 30: A passion for pollution prevention. *Green Chem.* **2023**, *25*, 1704–1728. [CrossRef]

48. Jain, N.; Mary, A.; Singh, T.; Gadiyaram, S.; Jose, D.A.; Naziruddin, A.R. Heteroleptic ruthenium(II) complexes featuring N-heterocyclic carbene-based C'N donor sets for solar energy conversion. *New J. Chem.* **2023**, *47*, 13476–13485. [CrossRef]

49. Kaneko, R.; Wu, G.; Sugawa, K.; Otsuki, J.; Islam, A.; Han, L.; Bedja, I.; Gupta, R.K. Cyclometalated ruthenium complexes with 6-(ortho-methoxyphenyl)-2,2'-bipyridine as panchromatic dyes for dye-sensitized solar cells. *J. Organomet. Chem.* **2017**, *833*, 61–70. [CrossRef]

50. Wu, G.; Kaneko, R.; Islam, A.; Zhang, Y.; Sugawa, K.; Han, L.; Shen, Q.; Bedja, I.; Gupta, R.K.; Otsuki, J. Thiocyanate-free asymmetric ruthenium(II) dye sensitizers containing azole chromophores with near-IR light-harvesting capacity. *J. Power Sources* **2016**, *331*, 100–111. [CrossRef]

51. Wu, G.; Kaneko, R.; Zhang, Y.; Shinozaki, Y.; Sugawa, K.; Islam, A.; Han, L.; Bedja, I.; Gupta, R.K.; Shen, Q.; et al. Neutral and anionic tetrazole-based ligands in designing novel ruthenium dyes for dye-sensitized solar cells. *J. Power Sources* **2016**, *307*, 416–425. [CrossRef]

52. Breivogel, A.; Wooh, S.; Dietrich, J.; Kim, T.Y.; Kang, Y.S.; Char, K.; Heinze, K. Anchor-Functionalized Push-Pull-Substituted Bis(tridentate) Ruthenium(II) Polypyridine Chromophores: Photostability and Evaluation as Photosensitizers. *Eur. J. Inorg. Chem.* **2014**, *16*, 2720–2724. [CrossRef]
53. Raboin, J.C.; Kirsch, G.; Beley, M. On the Way to Unsymmetrical Terpyridines Carrying Carboxylic Acids. *J. Heterocycl. Chem.* **2000**, *37*, 1077–1080. [CrossRef]

54. Woodward, C.P.; Coghlan, C.J.; Rüther, T.; Jones, T.W.; Hebing, Y.; Cordiner, R.L.; Dawson, R.E.; Robinson, D.E.J.E.; Wilson, G.J. Oligopyridine ligands possessing multiple or mixed anchoring functionality for dye-sensitized solar cells. *Tetrahedron* **2015**, *71*, 5238–5247. [CrossRef]

55. Shinpuku, Y.; Inui, F.; Nakai, M.; Nakabayashi, Y. Synthesis and characterization of novel cyclometalated iridium(III) complexes for nanocrystalline TiO₂-based dye-sensitized solar cells. *J. Photochem. Photobiol. A-Chem.* **2011**, *222*, 203–209. [CrossRef]

56. Vougioukalakis, G.C.; Stergiopoulos, T.; Kantonis, G.; Kontos, A.G.; Papadopoulos, K.; Stublla, A.; Potvin, P.G.; Falaras, P. Terpyridine- and 2,6-dipyrazinylpyridine-coordinated ruthenium(II) complexes: Synthesis, characterization and application in TiO₂-based dye-sensitized solar cells. *J. Photochem. Photobiol. A-Chem.* **2010**, *214*, 22–32. [CrossRef]

57. Ozawa, H.; Fukushima, K.; Sugiura, T.; Urayama, A.; Arakawa, H. Ruthenium sensitizers having an *ortho*-dicarboxyl group as an anchoring unit for dye-sensitized solar cells: Synthesis, photo- and electrochemical properties, and adsorption behavior to the TiO₂ surface. *Dalton Trans.* **2014**, *43*, 13208–13218. [CrossRef] [PubMed]

58. Rosero, W.A.A.; Guimaraes, R.R.; Matias, T.A.; Araki, K. Effect of Push-Pull Ruthenium Complex Adsorption Conformation on the Performance of Dye-Sensitized Solar Cells. *J. Braz. Chem. Soc.* **2020**, *31*, 2250–2264. [CrossRef]

59. Beley, M.; Bignozzi, C.A.; Kirsch, G.; Alebbi, M.; Raboin, J.-C. New ruthenium sisterpyridinyl complexes, as efficient sensitizers of nanocrystalline, TiO₂ films. *Inorg. Chim. Acta* **2001**, *318*, 197–200. [CrossRef]

60. da Silva, M.R.E.; Auvray, T.; Hanan, G.S. Synthesis of a novel bipyrimidine dicarboxylic acid ligand for the preparation of panchromatic ruthenium dyes. *Inorg. Chim. Acta* **2020**, *499*, 119194. [CrossRef]

61. Kisserwan, H.; Kamar, A.; Shoker, T.; Ghaddar, T.H. Photophysical properties of new cyclometalated ruthenium complexes and their use in dye sensitized solar cells. *Dalton Trans.* **2012**, *41*, 10643–10651. [CrossRef]

62. Constable, E.C.; Redondo, A.H.; Housecroft, C.E.; Neuburger, M.; Schaffner, S. Copper(I) complexes of 6,6'-disubstituted 2,2'-bipyridine dicarboxylic acids: New complexes for incorporation into copper-based dye sensitized solar cells (DSCs). *Dalton Trans.* **2009**, *33*, 6634–6644. [CrossRef] [PubMed]

63. Husson, J.; Beley, M.; Kirsch, G. A novel pathway for the synthesis of a carboxylic acid-functionalised Ru(II) terpyridine complex. *Tetrahedron Lett.* **2003**, *44*, 1767–1770. [CrossRef]

64. Jain, N.; Mary, A.; Manjunath, V.; Sakla, R.; Devan, R.S.; Jose, D.A.; Naziruddin, A.R. Ruthenium (II) Complexes Bearing Heteroleptic Terpyridine Ligands: Synthesis, Photophysics and Solar Energy Conversion. *Eur. J. Inorg. Chem.* **2021**, *2021*, 5014–5023. [CrossRef]

65. Duprez, V.; Biancardo, M.; Krebs, F.C. Characterisation and application of new carboxylic acid-functionalised ruthenium complexes as dye-sensitisers for solar cells. *Sol. Energy Mater. Sol. Cells* **2007**, *91*, 230–237. [CrossRef]

66. Koivisto, B.D.; Robson, K.C.D.; Berlinguette, C.P. Systematic Manipulation of the Light-Harvesting Properties for Tridentate Cyclometalated Ruthenium(II) Complexes. *Inorg. Chem.* **2009**, *48*, 9644–9652. [CrossRef]

67. Mongal, B.N.; Bhattacharya, S.; Mandal, T.K.; Datta, J.; Naskar, S. Synthesis, characterization and photovoltaic studies of 2,2';6',2''-terpyridine-based ruthenium complexes with phenylamino, anthranyl and furfuryl substitutions at the 4'-position. *J. Coord. Chem.* **2021**, *74*, 1382–1398. [CrossRef]

68. Das, D.; Sutradhar, S.; Singh, A.; Ghosh, B.N. Zinc-Terpyridine Based Chemosensor for Detection of Pyrophosphate Anion in Aqueous Medium. *Z. Anorg. Allg. Chem.* **2021**, *647*, 1234–1238. [CrossRef]

69. Manchand, P.S.; Belica, P.S.; Wong, H. Synthesis of 3,4,5-Trimethoxybenzaldehyde. *Synth. Commun.* **1990**, *20*, 2659–2666. [CrossRef]

70. Rao, D.V.; Stuber, F.A. An Efficient Synthesis of 3,4,5-Trimethoxybenzaldehyde from Vanillin. *Synthesis* **1983**, *4*, 308. [CrossRef]

71. Erofeev, Y.V.; Afanas'eva, V.L.; Glushkov, R.G. Synthetic routes to 3,4,5-trimethoxybenzaldehyde. *Pharm. Chem. J.* **1990**, *24*, 501–510. [CrossRef]

72. Mongal, B.N.; Bhattacharya, S.; Sengupta, S.; Mandal, T.K.; Datta, J.; Naskar, S.A. A novel ruthenium sensitizer with -Ome substituted phenyl-terpyridine ligand for dye sensitized solar cells. *Sol. Energy* **2016**, *134*, 107–118. [CrossRef]

73. Buckles, R.E.; Mock, G.V.; Locatell, L., Jr. Tiglic and Angelic Acids. *Chem. Rev.* **1955**, *55*, 659–677. [CrossRef]

74. Adeloye, A.O.; Olomola, T.O.; Adebayo, A.I.; Ajibade, P.A. A High Molar Extinction Coefficient Bisterpyridyl Homoleptic Ru(II) Complex with *trans*-2-Methyl-2-butoenoic Acid Functionality: Potential Dye for Dye-Sensitized Solar Cells. *Int. J. Mol. Sci.* **2012**, *13*, 3511–3526. [CrossRef]

75. Winter, A.; Schubert, U.S. Metal-Terpyridine Complexes in Catalytic Application- A Spotlight on the Last Decade. *ChemCatChem* **2020**, *12*, 2890–2941. [CrossRef]

76. Jarosz, P.; Du, P.; Schneider, J.; Lee, S.-H.; McCamant, D.; Eisenberg, R. Platinum(II) Terpyridyl Acetylide Complexes on Platinized TiO₂: Toward the Photogeneration of H₂ in Aqueous Media. *Inorg. Chem.* **2009**, *48*, 9653–9663. [CrossRef] [PubMed]

77. DeLucia, N.A.; Jystad, A.; Laan, K.V.; Tengco, J.M.M.; Caricato, M.; Vannucci, A.K. Silica Supported Molecular Palladium Catalyst for Selective Hydrodeoxygenation of Aromatic Compounds under Mild Conditions. *ACS Catal.* **2019**, *9*, 9060–9071. [CrossRef]

78. Boulogne, I.; Petit, P.; Ozier-Lafontaine, H.; Desfontaines, L.; Loranger-merciris, G. Insecticidal and antifungal chemicals produced by plants: A review. *Environ. Chem. Lett.* **2012**, *10*, 325–347. [CrossRef]

79. Sun, W.L.; Shahrajabian, M.H.; Cheng, Q. Anise (*Pimpinella anisum* L.), a dominant spice and traditional medicinal herb for both food and medicinal purposes. *Cogent Biol.* **2019**, *5*, 1673688. [CrossRef]
80. Macabeo, A.P.G.; Avila, J.A.; Alejandro, G.J.D.; Franzblau, S.G.; Kouam, S.F.; Hussain, H.; Krohn, K. Villarinol, a new Alkenoy-loxyalkenol Derivative from the Endemic Philippine Rubiaceae species *Villaria odorata*. *Nat. Prod. Commun.* **2012**, *7*, 779–780. [CrossRef]

81. Deng, W.P.; Zhang, H.X.; Wu, X.J.; Li, R.S.; Zhang, Q.H.; Wang, Y. Oxidative conversion of lignin and lignin model compounds catalyzed by CeO₂-supported Pd nanoparticles. *Green Chem.* **2015**, *17*, 5009–5018. [CrossRef]

82. Wu, Z.-Y.; Zhang, Q.-X.; Huang, L.-J.; Xu, Y.-J.; Tang, D.-L. Covalent immobilization of ruthenium polypyridyl complex on multi-walled carbon nanotube supports for oxygen evolution reaction in an alkaline solution. *J. Power Sources* **2021**, *488*, 229448. [CrossRef]

83. Chin, T.; Gao, Z.N.; Lelouche, I.; Shin, Y.G.K.; Purandare, A.; Knapp, S.; Isied, S.S. Molecular Recognition and Reactivity of Ruthenium(II) Bipyridine Barbituric Acid Guests in the Presence of Complementary Hosts: Ruthenium(II) Promoted Enolization of Barbituric Acids in Guest–Host Complexes. *J. Am. Chem. Soc.* **1997**, *119*, 12849–12858. [CrossRef]

84. Maggini, M.; Scorrano, G.; Prato, M. Addition of azomethine ylides to C60: Synthesis, characterization, and functionalization of fullerene pyrrolidines. *J. Am. Chem. Soc.* **1993**, *115*, 9798–9799. [CrossRef]

85. Ahangaran, F.; Navarchian, A.H. Recent advances in chemical surface modification of metal oxide nanoparticles with silane coupling agents; A review. *Adv. Colloid Interface Sci.* **2020**, *286*, 102298. [CrossRef]

86. Bahrami, K.; Khodaei, M.M.; Meibodi, F.S. Suzuki and Heck cross-coupling reactions using ferromagnetic nanoparticle-supported palladium complex as an efficient and recyclable heterogeneous nanocatalyst in sodium dodecylsulfate micelles. *Appl. Organometal. Chem.* **2017**, *31*, c3627. [CrossRef]

87. Khodaei, M.M.; Bahrami, K.; Meibodi, F.S. Ferromagnetic nanoparticle-supported copper complex: A highly efficient and reusable catalyst for three-component syntheses of 1,4-disubstituted 1,2,3-triazoles and C-S coupling of aryl halides. *Appl. Organometal. Chem.* **2017**, *31*, c3714. [CrossRef]

88. Sarabi, M.F.; Bezaatpour, A.; Mahmoudi, A. Anchoring of a terpyridine-based Mo(VI) complex on manganese ferrite as a recoverable catalyst for epoxidation of olefins under solvent-free conditions. *J. Coord. Chem.* **2021**, *74*, 1597–1612. [CrossRef]

89. Bahrami, K.; Targhan, H. A new strategy to design a graphene oxide supported palladium complex as a new heterogeneous nanocatalyst and application in carbon-carbon and carbon-heteroatom cross-coupling reactions. *Appl. Organometal. Chem.* **2019**, *33*, e4842. [CrossRef]

90. Wan, L.; Sun, X.; Shi, S.; Zhang, J.; Li, X.; Li, Z.; Guo, K. An efficient synthesis of N-substituted phtalimides using SiO₂-tpy-Nb as heterogeneous and reusable catalyst. *Catal. Commun.* **2017**, *88*, 30–34. [CrossRef]

91. Targhan, H.; Hassanpour, A.; Bahrami, K. Highly efficient polymer-stabilized palladium heterogeneous catalyst: Synthesis, characterization and application for Suzuki-Miyaura and Mizoroki-Heck coupling reactions. *Appl. Organometal. Chem.* **2019**, *33*, e5121. [CrossRef]

92. Klement, T.; Büchs, J. Itaconic acid—A biotechnological process in change. *Bioresour. Technol.* **2013**, *135*, 422–431. [CrossRef]

93. Targhan, H.; Hassanpour, A.; Sohrabnezhad, S.; Bahrami, K. Palladium Nanoparticles Immobilized with Polymer Containing Nitrogen-Based Ligand: A Highly Efficient Catalyst for Suzuki-Miyaura and Mizoroki-Heck Coupling Reactions. *Catal. Lett.* **2020**, *150*, 660–673. [CrossRef]

94. Yoo, D.-W.; Yoo, S.-K.; Kim, C.; Lee, J.-K. A novel mononuclear Fe(III) mono(terpyridine) complex having labile solvent ligands and its catalytic activity. *J. Chem. Soc. Dalton Trans.* **2002**, *21*, 3931–3932. [CrossRef]

95. Suzuka, T.; Kimura, K.; Nagamine, T. Reusable Polymer-Supported Terpyridine Palladium Complex for Suzuki-Miyaura, Mizoroki-Heck, Sonogashira, and Tsuji-Trost Reaction in Water. *Polymers* **2011**, *3*, 621–639. [CrossRef]

96. Kaskel, S. *The Chemistry of Metal-Organic Frameworks: Synthesis, Characterization, and Applications*; Wiley-VCH: Weinheim, Germany, 2016.

97. Batten, S.R.; Neville, S.M.; Turner, D.R. *Coordination Polymers: Design, Analysis and Application*; RSC Publishing: Cambridge, UK, 2008.

98. Schubert, U.S.; Eschbaumer, C. Macromolecules containing bipyridine and terpyridine metal complexes: Towards metallo-supramolecular polymers. *Angew. Chem. Int. Ed.* **2002**, *41*, 2892–2926. [CrossRef]

99. Etienne, S.; Beley, M. Preparation and study of ruthenium(II) 2,2'[:6',2'"-terpyridine complexes linked by an O-CH₂ spacer to thiophene moieties. *Inorg. Chem. Commun.* **2006**, *9*, 68–71. [CrossRef]

100. Manca, P.; Pilo, M.I.; Sanna, G.; Bergamini, G.; Ceroni, P.; Boaretto, R.; Caramori, S. Heteroleptic Ru(II)-terpyridine complex and its metal-containing conducting polymer: Synthesis and characterization. *Synth. Met.* **2015**, *200*, 109–116. [CrossRef]

101. Zhang, Z.; Chang, H.; Kang, Y.; Li, X.; Jiang, H.; Xue, B.; Wang, Y.; Lü, X.; Zhu, X. Water soluble Ln(III)-based metallopolymer with AIE-active and ACQ-effect lanthanide behaviors for detection of nanomolar pyrophosphate. *Sens. Actuator B-Chem.* **2019**, *282*, 999–1007. [CrossRef]

102. Huang, Y.; Feng, W.; Zhou, Z.; Zheng, H.; Zhao, Y.; Yan, H.; Lü, X. Tetraphenylethylene-based Eu³⁺-metallopolymers with aggregation-enhanced white emission for self-calibrating temperature sensing and white light-emitting diodes (WLEDs). *J. Mater. Chem. C* **2022**, *10*, 7586–7593. [CrossRef]

103. Friese, V.A.; Kurth, D.G. Soluble dynamic coordination polymers as a paradigm for materials science. *Coord. Chem. Rev.* **2008**, *252*, 199–211. [CrossRef]

104. Robb, M.G.; Brooker, S. Incorporation of Switchable Inorganic Building Blocks into Heterometallic Coordination Polymers. *Cryst. Growth Des.* **2023**, *23*, 1848–1859. [CrossRef]
105. Wang, W.; Xiao, Z.; Lin, H.; Wang, R.; Zhang, L.; Sun, D. Synthesis, structure, and properties of a 3D porous Zn(II) MOF constructed from a terpyridine-based ligand. *RSC Adv.* **2016**, *6*, 16575–16580. [CrossRef]

106. Zhang, J.; Yang, W.; Wu, X.-Y.; Zhang, L.; Lu, C.-Z. Synthesis, Photoluminescence, and Gas Adsorption Properties of a New Furan-Functionalized MOF and Direct Carbonization for Synthesis of Porous Carbon. *Cryst. Growth Des.* **2016**, *16*, 475–482. [CrossRef]

107. Constable, E.C.; Zhang, G.; Coronado, E.; Housecroft, C.E.; Neuburger, M. Not just size and shape: Spherically symmetrical $d^5$ and $d^{10}$ metal ions give different coordination nets with 4,2′:6′,4″-terpyridines. *CrystEngComm* **2010**, *12*, 2139–2145. [CrossRef]

108. Nijs, T.; Malzner, F.J.; Fatayer, S.; Wäckerlin, A.; Nowakowska, S.; Constable, E.C.; Housecroft, C.E.; Jung, T.A. Programmed assembly of 4,2′:6′,4″-terpyridine derivatives into porous, on-surface networks. *Chem. Commun.* **2015**, *51*, 12297–12300. [CrossRef] [PubMed]

109. Klein, Y.M.; Prescimone, A.; Constable, E.C.; Housecroft, C.E. 4,2′:6′,4″- and 3,2′:6′,3″-Terpyridines: The Conflict between Well-Defined Vectorial Properties and Serendipity in the Assembly of 1D-, 2D- and 3D-Architectures. *Materials* **2017**, *10*, 728. [CrossRef] [PubMed]

110. Khatua, S.; Goswami, S.; Biswas, S.; Tomar, K.; Jena, H.S.; Konar, S. Stable Multiresponsive Luminescent MOF for Colorimetric Detection of Small Molecules in Selective and Reversible Manner. *Chem. Mater.* **2015**, *27*, 5349–5360. [CrossRef]

111. Kharwar, A.K.; Konar, S. Exchange coupled Co(II) based layered and porous metal-organic frameworks: Structural diversity, gas adsorption, and magnetic properties. *Dalton Trans.* **2020**, *49*, 4012–4021. [CrossRef]

112. Liu, S.; Tang, Z. Polyoxometalate-based functional nanostructured films: Current progress and future prospects. *Nano Today* **2010**, *5*, 267–281. [CrossRef]

113. Wang, S.-S.; Yang, G.-Y. Recent Advances in Polyoxometalate-Catalyzed Reactions. *Chem. Rev.* **2015**, *115*, 4893–4962. [CrossRef]

114. Walsh, J.J.; Bond, A.M.; Forster, R.J.; Keyes, T.E. Hybrid polyoxometalate materials for photo(electro-) chemical applications. *Coord. Chem. Rev.* **2016**, *306*, 217–234. [CrossRef]

115. Verissimo, M.I.S.; Evtuguin, D.V.; Gomes, M.T.S.R. Polyoxometalate Functionalized Sensors: A Review. *Front. Chem.* **2022**, *10*, 840657. [CrossRef] [PubMed]

116. Santoni, M.-P.; Pal, A.K.; Hanan, G.S.; Proust, A.; Hasenknoph, B. Discrete Covalent Organic-Inorganic Hybrids: Terpyridine Functionalized Polyoxometalates Obtained by a Modular Strategy and Their Metal Complexation. *Inorg. Chem.* **2011**, *50*, 6737–6745. [CrossRef]

117. Liu, Y.; Deng, W.; Meng, Z.; Wong, W.-Y. A Tetrakis(terpyridine) Ligand Based Cobalt(II) Complex Nanosheet as a Stable Dual Ion Battery Cathode Material. *Small* **2020**, *16*, 1905204. [CrossRef]

118. Zhu, H.; Liao, S.; Bian, R.; Su, B.; Ding, X.; Li, M.; Ge, S.; Zhang, H.; Liu, Q. An iron supramolecular compound containing terpyridine polycarboxylic acid for high performance lithium-ion batteries. *Inorg. Chim. Acta* **2022**, *535*, 120848. [CrossRef]

119. Gu, C.; Li, J.; Liu, J.-P.; Wang, H.; Peng, Y.; Liu, C.-S. Conferring supramolecular guanosine gel nanofiber with ZIF-67 for high-performance oxygen reduction catalysis in rechargeable zinc-air batteries. *Appl. Catal. B-Environ.* **2021**, *286*, 119888. [CrossRef]

120. Yuan, J.; Dong, H.; Wang, B.; Qiu, M.; Liu, Z.; Wu, X.; Zhong, S.; Tong, G.; Chen, Z.; Zhang, J.; et al. Coordination polymer-reinforced composite polymer electrolyte for all-solid-state Li-metal batteries. *Chem. Eng. J.* **2024**, *487*, 150489. [CrossRef]

121. Mondal, S.; Yoshida, T.; Maji, S.; Ariga, K.; Higuchi, M. Transparent Supercapacitor Display with Redox-Active Metallo-Supramolecular Polymer Films. *ACS Appl. Mater. Interfaces* **2020**, *12*, 16342–16349. [CrossRef]

122. Kyriakopoulos, G.L.; Arabatzis, G. Electrical energy storage systems in electricity generation: Energy policies, innovative technologies, and regulatory regimes. *Renew. Sust. Energ. Rev.* **2016**, *56*, 1044–1067. [CrossRef]

123. Zhang, H.D.; Zhu, H.T.; Bian, R.R.; Liu, Q.; Liao, S.Y. Heterometallic-organic frameworks containing Fe(II) nodes as high-performance anode materials for Li-ion batteries. *J. Solid State Electrochem.* **2024**. [CrossRef]

124. Pan, S.-Y.; Chiang, P.-C.; Pan, W.; Kim, H. Advances in state-of-art valorization technologies for captured CO₂ toward sustainable carbon cycle. *Crit. Rev. Environ. Sci. Technol.* **2018**, *48*, 471–534. [CrossRef]

125. Arana, C.; Keshavarz, M.; Potts, K.T.; Abruna, H.D. Electrocatalytic reduction of CO₂ and O₂ with electropolymerized films of vinyl-terpyridine complexes of Fe, Ni and Co. *Inorg. Chim. Acta* **1994**, *225*, 285–295. [CrossRef]

126. Gautam, P.; Srivastava, V. Synthesis and Catalytic Application of Ru-Deposited Magnetic Nanoparticles for the Selective Hydrogenation of CO₂ Gas. *Lett. Org. Chem.* **2022**, *19*, 705–710. [CrossRef]

127. Lam, E.; Reisner, E. A TiO₂-Co(terpyridine)₂ Photocatalyst for the Selective Oxidation of Cellulose to Formate Coupled to the Reduction of CO₂ to Syngas. *Angew. Chem. Int. Ed.* **2021**, *60*, 23306–23312. [CrossRef] [PubMed]

128. Faisal, M.; Rehman, Z.U.; ul Ain, Q.; Saeed, A. Terpyridine-Pr-Fe₃O₄@boehmite nanoparticles; a novel and highly effective magnetic nanocatalyst for preparation of cyclic carbonates from carbon dioxide and epoxides under solventless conditions. *Mater. Chem. Phys.* **2019**, *231*, 272–280. [CrossRef]

129. Xang, X.; Li, J.; Kou, M.; Dou, W.; Bai, D.; Tang, X.; Tang, Y.; Liu, W. Dual-Function Precious-Metal-Free Metal-Organic Framework for Photocatalytic Conversion and Chemical Fixation of Carbon Dioxide. *Inorg. Chem.* **2023**, *62*, 19015–19024.

130. Zhou, P.; Zhou, X.; Song, Z.; Shao, D.; Wang, D. Metal-organic frameworks with Lewis acid-base sites as highly efficient catalyst for the cycloaddition of carbon dioxide. *J. Solid State Chem.* **2024**, *331*, 124500. [CrossRef]

131. Kim, D.; Bhattacharjee, S.; Lam, E.; Casadevall, C.; Rodriguez-Jimenez, S.; Reisner, E. Photocatalytic CO₂ Reduction Using Homogeneous Carbon Dots with a Molecular Cobalt Catalyst. *Small* **2024**, 2400057. [CrossRef]
132. Verma, P.; Singh, A.; Rahimi, F.A.; Sarkar, P.; Nath, S.; Pati, S.K.; Maji, T.K. Charge-transfer regulated visible light driven photocatalytic H₂ production and CO₂ reduction in tetrathiafulvalene based coordination polymer gel. *Nat. Commun.* **2021**, *12*, 7313. [CrossRef]

133. Zhao, J.; Ziaratti, A.; Rosspeintner, A.; Bürgi, T. Anchoring of Metal Complexes on Au<sub>25</sub> Nanocluster for Enhanced Photocoupled Electrocatalytic CO<sub>2</sub> Reduction. *Angew. Int. Ed.* **2024**, *63*, e202316649. [CrossRef]

134. Wang, R.; Both, S.K.; Geven, M.; Calucci, L.; Forte, C.; Dijkstra, P.J.; Karpieren, M. Kinetically stable metal ligand charge transfer complexes as crosslinks in nanogels/hydrogels: Physical properties and cytotoxicity. *Acta Biomater.* **2015**, *26*, 136–144. [CrossRef] [PubMed]

135. Ferraro, G.; Pica, A.; Petruk, G.; Pane, F.; Amoresano, A.; Cilibrizzi, A.; Vilar, R.; Monti, D.M.; Merlino, A. Preparation, structure, Cytotoxicity and Mechanism of Action of ferritin-Pt(II) Terpyridine Compound Nanocomposites. *Nanomedicine* **2018**, *13*, 2995–3007. [CrossRef] [PubMed]

136. Wild, A.; Babiuch, K.; König, M.; Winter, A.; Hager, M.D.; Gottschaldt, M.; Prokon, A.; Schubert, U.S. Synthesis of a glycopolymeric PtII carrier and its induction of apoptosis in resistant cancer cells. *Chem. Commun.* **2012**, *48*, 6357–6359. [CrossRef]

137. Viale, M.; Bertole, N.; Panebianco, R.; Vecchio, G. Terpyridine Functionalized Cyclodextrin Nanoparticles as Carriers for Doxorubicin: Analysis of In Vitro Antiproliferative Activity. *Anticancer Res.* **2023**, *43*, 5409–5414. [CrossRef] [PubMed]

138. Hassan, E.A.; Hassan, M.L. Rice straw nanofibrillated cellulose films with antimicrobial properties via supramolecular route. *Ind. Crop Prod.* **2016**, *93*, 142–151. [CrossRef]

139. Gao, L.; Hou, Y.; Wang, H.; Li, M.; Ma, L.; Chu, Z.; Donskyi, I.S.; Haag, R. A Metal-Ion-Incorporated Mussel-Inspired Poly(Vinyl Alcohol)-Based Polymer Coating Offers Improved Antibacterial Activity and Cellular Mechanoresponse Manipulation. *Angew. Chem. Int. Ed.* **2022**, *61*, e202201563. [CrossRef] [PubMed]

140. Jacquet, M.; Izzo, M.; Osella, S.; Kozdra, S.; Michalowski, P.P.; Golowicz, D.; Kazimierczuk, K.; Gorkowski, M.T.; Lewera, A.; Teodorczyk, M.; et al. Development of a universal conductive platform for anchoring photo- and electroactive proteins using organometallic terpyridine molecular wires. *Nanoscale* **2021**, *13*, 9773–9787. [CrossRef] [PubMed]

141. Dai, W.; Chen, G.; Wang, X.; Zhen, S.; Huang, C.; Zhan, L.; Li, Y. Facile synthesis of dual-ligand europium-metal organic gels for ratiometric electrochemiluminescence detecting I27L gene. *Biosens. Bioelectron.* **2024**, *246*, 115863. [CrossRef] [PubMed]

**Disclaimer/Publisher's Note:** The statements, opinions and data contained in all publications are solely those of the individual author(s) and contributor(s) and not of MDPI and/or the editor(s). MDPI and/or the editor(s) disclaim responsibility for any injury to people or property resulting from any ideas, methods, instructions or products referred to in the content.